HAL Id: hal-01006704
Submitted on 27 Jan 2018
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Coupling Moisture Diffusion and Internal Mechanical
States in Polymers - A Thermodynamical Approach
Bun Eang Sar, Sylvain Fréour, Peter Davies, Frédéric Jacquemin
To cite this version:
Bun Eang Sar, Sylvain Fréour, Peter Davies, Frédéric Jacquemin. Coupling Moisture Diffusion and
Internal Mechanical States in Polymers - A Thermodynamical Approach. European Journal of
Me-chanics - A/Solids, Elsevier, 2012, 36, pp.38-43. �10.1016/j.euromechsol.2012.02.009�. �hal-01006704�
Coupling moisture diffusion and internal mechanical states in
e A thermodynamical approach
, S. Fréoura
, P. Daviesb
, F. Jacquemina,*
aInstitut de Recherche en Génie Civil et Mécanique, UMR CNRS 6183, LUNAM Université, Université de Nantes, Ecole Centrale de Nantes, 37 Bd de l’Université, BP 406,
44602 Saint-Nazaire, France
bService Matériaux et Structures, IFREMER, Centre de Brest, B.P. 70, 29280 Plouzané, France
Keywords: Hygromechanical coupling, Moisture absorption, Thermodynamical approach
A thermodynamical approach, based on the deﬁnition of the chemical potential of water, is used in order to establish a model coupling the diffusion of moisture to the mechanical behaviour of a polymer. The model takes into account the evolution, occurring during the diffusion process, of both the density of the polymer and its maximum moisture absorption capacity. The approach developed is applied to symmetric loading cases, in terms of relative humidity and external pressure. The model, established in the present work, provides the water content proﬁles through the thickness of the polymer throughout the transient phase of the diffusion process. The numerical results obtained show the signiﬁcant effect of an external pressure on the kinetics of moisture diffusion in polymers.
Fiber reinforced organic matrix composites are being increas-ingly used for aircraft, marine and civil engineering structural applications. Such composite structures are often subjected to humid environments during their service life (Jedidi et al., 2005). Organic matrix composites do absorb signiﬁcant amount of water when exposed to moisture. Many authors have reported that hygro-thermal ageing could induce a loss of the mechanical stiffness and/ or strength of organic matrix composites (Patel et al., 2002). Moreover, the constituents of composite structures exhibit heterogeneous coefﬁcients of moisture expansion (CME) and maximum moisture absorption capacity. As a consequence, multi-scale mechanical behaviour proﬁles arise during the hygroscopic loading of organic matrix composites. According to the literature, the resulting mechanical states can eventually induce damage (Perreux and Suri, 1997; Weitsman and Elahi, 2000). Therefore, considerable research efforts have been made in order to develop analytical models to predict the multi-scale mechanical states occurring during both the transient stage and the permanent regime of the moisture diffusion process in organic matrix composites subjected to hygro-mechanical loads (Jacquemin and Vautrin, 2002; Fréour et al., 2005). In thisﬁeld of research, the most recent investigations (Aboudi and Williams, 2000; Derrien
and Gilormini, 2009;Youssef et al., 2009,2011) focus upon taking into account, in the theoretical approaches, various features of hygro-mechanical coupling, observed during experimental studies, and in particular the dependence of both the moisture diffusion coefﬁcient and the maximum moisture absorption capacity on the mechanical states (strains and stresses) (Marom and Broutman, 1981; Neumann and Marom, 1986, 1987). These models aim eventually to enable the prediction of the long-term durability of composite structures subjected to hygroscopic loads.
The purpose of this study is to establish a model coupling the diffusion of moisture to the mechanical states by a thermodynamical approach, based on the expression satisﬁed by the chemical potential of water. Moreover, the present study aims to consider additional factors that have not yet been taken into account in the pioneering works of Derrien and Gilormini (Derrien and Gilormini, 2009), such as the evolution of the polymer density as a function of the mechanical states, which occurs in practice during the moisture diffusion process.
2. Conservation of mass equation
The uncoupled law of Fick is classically used for modelling the diffusion of moisture in organic matrix composites. The adjective “uncoupled” refers to the fact that the model disregards any effect due to the mechanical states on the moisture diffusion process. However, the experimental investigation reported in Gilat and Broutman (1978)shows that an anomalous sorption process (i.e. it deviates from the classical Fickian behaviour) takes place in
* Corresponding author.
practice. According toWeitsman (1990), the anomalies could be explained by coupled constitutive equations, based on the princi-ples of continuum mechanics and irreversible thermodynamics.
In practice, the coupled method relates theﬂux of moisture to the chemical potential~
Ji ¼ DCRTV~
Where D is the diffusion coefﬁcient in [mm2/s], C is the moisture content in [%], R is the ideal gas constant in [kJ/(mol K)], T is the temperature in [K].
The coupled diffusion equation which expresses the law of mass conservation is given byLarché and Cahn (1982):
vtþ Ji;i ¼ 0 (2)
3. Chemical potential
The chemical potential of water
m~w is deﬁned as the partial
derivative of free energy of Helmholtz, F ¼ F0þ nfw(C) þ V3W, with
respect to the amount of water nw. Where F0is the free energy of
the dry stress-free polymer, fw(C) is the variation of the free energy
per mole of dry polymer, due to the addition of water when the polymer is free to swell, n and V3 are respectively the amount of
polymer and its volume at any stage, whereas W denotes the hygro-elastic strain energy (Derrien and Gilormini, 2009):
mw C¼ vF vnw ¼ vF vC vC vnw (3)
The moisture content in the polymer is calculated through C ¼ (nw
ustand for respectively the molar mass
of water and polymer.
The hygro-elastic strain energy written as a function of both the bulk modulus k and shear modulus G, is deﬁned by:
W ¼ 1
el ¼ k
2þGe : e (4)
Where 3elis the elastic strain, 3 being the total strain, e the
devia-toric strain tensor.
hdenotes the coefﬁcient of moisture expansion of the polymer.
Introducing fw0ðCÞ ¼ v½fwðCÞ=vC, one obtains the following
expression for the derivative of the Helmholtz free energy with respect to the moisture content:
vF vC ¼ vF0 vCþ nfw0ðCÞ þ V3 vW vC þ W vV3 vC (5)
Let us assume that
i). following the historical hypotheses accounted inDerrien and Gilormini (2009), the derivative of polymer volume with respect to moisture content is considered as negligible, i.e. vV3/vC ¼ 0,
ii). the bulk modulus k, and the shear modulus G, do not depend on the moisture content (vk/vC ¼ vG/vC ¼ 0) and
iii). the derivative of the strain tensor trace by the moisture content is also negligible:v (tr3)/vC ¼ 0.
Accounting for above the approximations i) to iii) in (8, 10)
yields vF vC ¼ nfw0ðCÞ þ V3 v vC kðCÞ 2 ðtr3 3
hCÞ 2þGe : e ’
The chemical potential canﬁnally be written as,
mw C ¼
uf 0 wðCÞ þ kðtr3 3
m0 denotes the chemical
potential of water in the strain-free polymer, whereas the reference moisture content is given by C0.
During the moisture diffusion process, we take into account the evolution of the volume occupied by the polymer, and the resulting variation of its density, through
¼ tr3 þ 1 (8)
Where V3, V0,
r0stand respectively for the polymer volume and
its density at present and initial states.
Assuming the mechanical properties of the polymer to be independent of both the mechanical states and the moisture content, the chemical potential can be written as,
mwðC; tr3Þ ¼
m0þ RT lnCC 0 3
r0 ðtr 3 3
hCÞðtr3 þ 1Þ (9) 4. Hygroscopic pressure
The hygro-elastic Hooke’s law is:
3ij ¼ 1þ
nstands for Poisson’s ratio, E for Young’s modulus, and
dij ¼ f1 if i ¼ j0 if isj .
The BeltramieMichell equation leads to:
dijC;kkþ C;ij ¼ 0 (11)
Furthermore, introducing the Laplacian operator
D, one can write:
¼ 0 (12)
In the present case, a hydrostatic external pressure Pex is assumed to be applied at the boundary of a cubic element, so that the total pressure is P ¼ Pex þ Pis where the hygroscopic pressure to be determined is denoted by Pis. As a result, tr
sij¼ 3P. Besides,
As a consequence, the hygroscopic pressure depends on the moisture content through:
hDC (13) Where,
aA0 ¼ 2E 3ð1
nÞ (14) A0 ¼ 3
r0 (15) 5. Equation of model
The constitutive equation is obtained by using the mass conservation Eq.(2)in which the chemical potential of water has been written as a function of the trace of the strains and the
vC vt ¼ D RTdiv h Cgrad !~
mwðC; tr3Þ i (16) Since grad !~
mwðC; tr3Þ ¼ v~
mw vCgrad ! C þv~vtr
mw 3grad ! tr3 (17) v~
mw vC ¼ RT C þ 9
r0 ðtr 3 þ 1Þ (18) v~
mw vtr3 ¼ 3k
r0 ð2tr 3 3
hC þ 1Þ (19)
Therefore the Eq.(16)could be written as follows,
vC vt ¼ Ddiv grad !C þ9
r0 Cðtr 3 þ 1Þgrad !C 3k
r0 ð2tr 3 3
hC þ 1ÞC grad !tr3 (20) This implies, vC vt ¼ D
r0 Cðtr 3 þ 1Þ
r0 grad !½Cðtr3 þ 1Þ grad !C 3k
r0 ð2tr3 3
hC þ 1Þ C
r0 grad ! ½ð2tr3 3
hC þ 1ÞCgrad !tr3 ð21Þ
Since the trace of the strain in term of the pressure load is given by,
tr3 ¼ 3ðPex þ PisÞ
3k þ 3
This implies the gradient of strain trace can be written as follows,
grad !tr3 ¼ ðgrad
Pexþ grad !PisÞ
k þ 3
Knowing that the gradient of external pressure is given by,
grad !Pex¼ 0 (24)
6. Towards an explicit solution: the case of an unidirectional moisture diffusion
In order toﬁnd an explicit solution to relation(21), an unidi-rectional moisture diffusion is assumed to occur along x axis. As a result, the solution of Eq.(13)satisﬁes,
Pisx; t ¼
hCðx; tÞ þ k1ðtÞx þ k2ðtÞ (25)
The constants k1(t) and k2(t) are deduced from the equilibrium
conditions in which L is the dimension along the x axis,
ZL 0 Pisðx; tÞdx ¼ 0 (26) ZL 0 Pisðx; tÞxdx ¼ 0 (27)
Theﬁnal form of Eq.(13)is given by:
Pisðx; tÞ ¼
hðCðx; tÞ CðtÞÞ (28) Where CðtÞ ¼ 1 L ZL 0 Cðx; tÞdx (29)
As a result, the gradient of the hygroscopic pressure is given by,
grad ! Pis ¼ vxv
hðCðx; tÞ CðtÞÞ ¼
hvC vx (30)
It should be noted that CðtÞ only depends on the time (i.e., it is independent of the position), thus its derivative with respect to the position is obviously zero:vCðtÞ=vx ¼ 0.
So, the strain trace gradient(23)can be written from(24, 30)as equal to grad ! tr3 ¼ 3A0k
hvC vx (31)
Similarly, the Laplacian of the strain trace will be given by,
Dtr3 ¼ divðgrad !tr3Þ ¼ div 3A0k
hvC vx ¼3A0k
Introducing the relations(31)and(32)into the Eq.(26), enables the model’s fundamental constitutive equation to be obtained:
vC vt ¼ D " 1þ V1
h2C þ V2
h3C2v 2C vx2þ
h2ðV 3þ V4CÞ vC vx 2# (33) Where: V1 ¼ 3A0kCtr3 þ 2
a(34) V2 ¼ 9A0k 3
a(35) V3 ¼
a3A0ktr3 þ 2
atr3 (36) V4 ¼ 9
hA0k þ 3
ha2 A0k (37)
One should notice that the relation (33) merges with the constitutive law of the model, neglecting the volume change, proposed byDerrien and Gilormini (2006)which is recovered by taking V1¼ V3¼
aand V2¼ V4¼ 0.
7. Boundary condition
The boundary condition is obtained by equating the chemical potential of water in humid air,^
mw ¼ ^
m0þ RTlnðpw=p0Þ (where ^
is the chemical potential of water in humid air at the reference pressure p0, the partial pressure of water being pw) with the
generalized chemical potential of the polymer. The boundary condition is obviously only satisﬁed at the speciﬁc position xb
denoting the boundary between the ambientﬂuid and the polymer. Let us denote by P (xb, t) the pressure experienced at the
boundary, and C (xb, t) the corresponding moisture content. The
chemical potential(9)written in terms of the pressure reads,
m0þ RTlnCðxb; tÞC0 þ 3
r0 Pðxb; tÞ k ð Pðxb; tÞ þ 3
hkCðxb; tÞ þ kÞ (38)
So the equality of these two chemical potentials leads to ^
m0þ RTlnpwp0 ¼
m0þ RTlnCðxb; tÞC0 þ 3
r0 Pðxb; tÞ k ð Pðxb; tÞ þ 3
hkCðxb; tÞ þ kÞ (39) Then, Cðxb; tÞ pw ¼ C0 p0e ^ m0 m0 RT eA0 h k ðPðxb;tÞ23hkCðxb;tÞPðxb;tÞkPðxb;tÞÞ (40) Henry’s law is introduced to deﬁne sorption isotherm: the moisture at saturation is given by Cs¼ Spwwhere S is the solubility
of water given by S ¼ ðC0=p0Þeð^m0m0Þ=RT.
Cðxb; tÞ ¼ SpweA0khðPðxb;tÞ23hkCðxb;tÞPðxb;tÞkPðxb;tÞÞ (41)
To simplify in order to solve Eq.(41), the following assumption is considered to be satisﬁed: jðA0
h=kÞðPðxb; tÞ2 3
hkCðxb; tÞPðxb; tÞ
As a result, expression(41)simpliﬁes as follows,
Cðxb;tÞ ¼ Spw 1þA0
Through(42), we then get,
Cðxb; tÞ ¼ Spw1þ A0
hk Pðxb; tÞ2kPðxb; tÞ 1þ 3
h2A0Pðx b; tÞSpw (43)
The total pressure at the boundary position xbis given by,
Pðxb; tÞ ¼ Pis þ Pex ¼ A0
h½Cðxb; tÞ CðtÞ þ Pex (44)
Cðxb; tÞ ¼ CðtÞ þPðxb; tÞ Pex
Pðxb; tÞ Pex
hþ CðtÞ ¼ Spw1þ A0
hk Pðxb; tÞ2kPðxb; tÞ 1þ 3
h2A0Pðx b; tÞSpw (46)
The relation (46) above leads to the following equation as a function of the variable P (xb, t):
a1Pðxb; tÞ2þa2Pðxb; tÞ þ a3 ¼ 0 (47) Where a1 ¼ Spe
ak (48) a2 ¼ 1 3
ah2Spw (49) a3 ¼
hðCðtÞ SpwÞ Pex (50)
The single solution of Eq.(47)having a physical meaning is
Pðxb; tÞ ¼a2þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 2 4a1a3 q 2a1 (51)
In expression(51), by replacing P (xb, t) with the form(44), we
obtain, Cðxb; tÞ ¼ 1
h0 @a2þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 2 4a1a3 q 2a1 Pex 1 A þ CðtÞ ¼
h0 B B B B @ a2þ a2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 4a1a3 a2 2 s 2a1 Pex 1 C C C C Aþ CðtÞ (52)
In the case of the amountða1a3Þ=a22/0 the following
approxi-mation is considered to be satisﬁed
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 4a1a3 a2 2 s ¼ 1 2a1a3 a2 2 (53)
As a consequence, expression(52)reduces to:
Cðxb; tÞ ¼ CðtÞ A0
aha3 a2þ Pex (54)
Finally the boundary condition, in the case of a symmetrical hygro-mechanical loading, can be written as:
Cðxb; tÞ ¼ Spw 1þ A0
h2CðtÞ ð3A0Pex 3
aÞ 1 ð3A0Pex 3
h2Spw (55) 8. Numerical results
The numerical simulations correspond to a 4 mm thick plate made of epoxy resin whose Young modulus is 3.65 GPa and Pois-son’s ratio is 0.36. The polymer plate is subjected to moisture diffusion while experiencing a hydrostatic pressure load.
Fig. 1a shows the time-dependent evolution of the macroscopic (average) moisture content, as a function of the CME:
h¼ 0.6 or
h¼ 2, at an imposed pressure of 1 MPa. Increasing CME reduces the maximum moisture absorption capacity of the polymer as indicated by the evolution of the average moisture content in the steady state. Besides, Fig. 1a displays a comparison between the results predicted according to the present work and the model previously proposed byDerrien and Gilormini (2006)throughout the diffusion process. According to Fig. 1a, the discrepancies between the models signiﬁcantly increase with the coefﬁcient of moisture expansion. In particular, in the steady state, the maximum absorption capacity deduced from the boundary conditions differs depending on the considered model. Eventually, both the predicted maximum moisture absorption capacity and the apparent moisture diffusion coefﬁcient may vary whether the volume change is accounted for or neglected, instead.
The evolution of the moisture content proﬁles through the thickness of the plate during the transient stage of the diffusion
process is shown onFig. 1b for the case of a symmetrical pressure of 1 MPa and
According toFig. 1b, the moisture content at the boundary with humid air varies signiﬁcantly throughout the transient regime. This means that the maximum moisture absorption capacity does not immediately reach its ultimate value. This effect comes from the dependence of the boundary condition on the mechanical strain experienced by the polymer, the magnitude of which changes considerably during the transient part of the diffusion process, due to the hygroscopic swelling. The results obtained are consistent with those published in reference (Youssef et al., 2009).
Fig. 2shows the effect induced by the application of an external pressure, varying from 1 MPa to 20 MPa, on the time-dependent moisture content. The Coefﬁcients of Moisture Expansion used in order to obtain the results depicted onFig. 2a and b are respectively equal to 0.6 and 2. According to Fig. 2a, an increased applied pressure signiﬁcantly reduces the diffusion of moisture at the boundary.Fig. 2b shows that this effect increases with the CME.
Fig. 3shows that the maximum moisture absorption capacity reached in the steady state depends almost linearly on the applied pressure. The results are consistent withCai and Weistman (1994).
The aim of the present work is to establish a model enabling the moisture diffusion within polymers under external load (symmetric moisture and pressure conditions) to be predicted. The moisture sorption results from coupled hygro-mechanical phenomena. The model developed here is theﬁrst enriched one, following many previous studies based on empirical approaches such as a the free-volume theory (Neumann and Marom, 1986;Youssef et al., 2009,
2011). In contrast with previous work based on the thermody-namical approach, such as (Derrien and Gilormini, 2009), the present model accounts for the dependence of the polymer density on the mechanical states, which was previously neglected. The simulations reproduce the expected evolutions, as a function of the applied external pressure, of the maximum moisture absorption capacity. These results are compatible with results from published experimental investigations (Wan et al., 2005).
In future works, realistic evolutions of the hygro-mechanical properties (i.e. the elastic moduli and coefﬁcient of moisture expansion), occurring during the diffusion process, will be taken into account. Besides, sorptionedesorption case showing a hysteresis effect is an interesting feature occurring in practice in epoxy resin and its composites (Henson and Weitsman, 1986). This ﬁeld of research is under investigation by the authors: ongoing experimental studies should provide results to be compared with the numerical
Fig. 2. Effect of applied pressure on the average moisture content a).h¼ 0.6, b).h¼ 2.
Fig. 3. Maximum steady state moisture absorption capacity, as a function of the applied external load.
predictions. Finally, the model presented in this communication will be extended to the case of polymer matrix composites.
Aboudi, J., Williams, T.O., 2000. A coupled micro-macromechanical analysis of hygrothermoelastic composites. International Journal of Solids and Structures 37, 4149e4179.
Cai, L.-W., Weistman, Y., 1994. Non-ﬁckian moisture diffusion in polymeric composite. Journal of Composite Materials 28, 130e154.
Derrien, K., Gilormini, P., 2006. Interaction between stress and diffusion in poly-mers. Defect and Diffusion Forum 258e260, 447e452.
Derrien, K., Gilormini, P., 2009. The effect of moisture-induced swelling on the absorption capacity of transversely isotropic elastic polymer-matrix compos-ites. International Journal of Solids and Structures 46, 1547e1553.
Fréour, S., Jacquemin, F., Guillén, R., 2005. On an analytical self-consistent model for internal stress prediction inﬁber-reinforced composites submitted to hygroe-lastic load. Journal of Reinforced Phygroe-lastics and Composites 24, 1365e1377. Gilat, O., Broutman, L.J., 1978. Effect of external stress on moisture diffusion and
degradation in a graphite reinforced epoxy laminate. ASTM STP 658, 61e83. Henson, M.C., Weitsman, Y., 1986. Stress effects on moisture transport in an epoxy
resin and its composites. In: Kawaba, K., et al. (Eds.), Composites’ 86: Recent Advances in Japan and the United States, pp. 775e783.
Jacquemin, F., Vautrin, A., 2002. A closed-form solution for the internal stresses in thick composite cylinders induced by cyclical environmental conditions. Composite Structures 58, 1e9.
Jedidi, J., Jacquemin, F., Vautrin, A., 2005. Design of accelerated hygrothermal cycles on polymer matrix composites in the case of a supersonic aircraft. Composite Structures 68, 429e437.
Larché, F.C., Cahn, J.W., 1982. The effect of self-stress on diffusion in solid. Acta-Metallurgica 30, 1835e1845.
Marom, G., Broutman, L.J., 1981. Moisture penetration into composites under external stress. Polymer Composites 2, 132e136.
Neumann, S., Marom, G., 1986. Free-volume dependent moisture diffusion under stress in composite materials. Journal of Materials Science 21, 26e30.
Neumann, S., Marom, G., 1987. Prediction of moisture diffusion parameters in composite materials under stress. Journal of Composite Materials 21, 68e80.
Patel, B.P., Ganapathi, M., Makhecha, D.P., 2002. Hygrothermal effects on the structural behaviour of thick composite laminates using higher-order theory. Composite Structures 56, 25e34.
Perreux, D., Suri, C., 1997. A study of the coupling between the phenomena of water absorption and damage in glass/epoxy composite pipes. Composites Science and Technology 57, 1403e1413.
Wan, Y.Z., Wang, Y.L., Huang, Y., He, B.M., Han, K.Y., 2005. Hygrothermal aging behaviour of VARTMed three-dimensional braided carboneepoxy composites under external stresses. Composites Part A 36, 1102e1109.
Weitsman, Y.J., Elahi, M., 2000. Effects ofﬂuids on the deformation, strength and durability of polymeric composites e an overview. Mechanics of Time-Dependent Materials 4, 107e126.
Weitsman, Y.J., 1990. Moisture in composites: sorption and damage. In: Reifsnider, K.L. (Ed.), Fatigue of Composite Materials. Elsevier Science Publisher, pp. 385e429.
Youssef, G., Fréour, S., Jacquemin, F., 2009. Stress-dependent moisture diffusion in composite materials. Journal of Composite Materials 43, 1621e1637. Youssef, G., Jacquemin, F., Fréour, S., 2011. Radial Pressure and thickness effects on
the moisture diffusion in hollow composite cylinders. Polymer Composites 32 (6), 960e966.